1. Compiled By: Prof G B Rathod BVM Engineering College ET Department V V Nagar-Gujarat-India-388120 Email: email@example.com Gujarat Technological University Subject: VLSI Technology & Design Code:2161101 Topic_2_Fabrication of MOSFET
2. Outlines Introduction Fabrication Process flow: Basic steps C-MOS n-Well Process Layout Design rules full custom mask layout design Outcomes references 1/23/2016BVM ET2
3. Introduction In this chapter, the fundamentals of MOS chip fabrication will be discussed and the major steps of the process flow will be examined. It is not the aim of this chapter to present a detailed discussion of silicon fabrication technology, which deserves separate treatment in a dedicated course. Rather, the emphasis will be on the general outline of the process flow and on the interaction of various processing steps, which ultimately determine the device and the circuit performance characteristics. The following chapters show that there are very strong links between the fabrication process, the circuit design process and the performance of the resulting chip. Hence, circuit designers must have a working knowledge of chip fabrication to create effective designs and in order to optimize the circuits with respect to various manufacturing parameters. 1/23/2016BVM ET3
4. Introduction Also, the circuit designer must have a clear understanding of the roles of various masks used in the fabrication process, and how the masks are used to define various features of the devices on-chip. The following discussion will concentrate on the well-established CMOS fabrication technology, which requires that both n-channel (nMOS) and p-channel (pMOS) transistors be built on the same chip substrate. To accommodate both nMOS and pMOS devices, special regions must be created in which the semiconductor type is opposite to the substrate type. These regions are called wells or1/23/2016BVM ET4
5. Introduction A p-well is created in an n-type substrate or, alternatively, an n- well is created in a p-type substrate. In the simple n-well CMOS fabrication technology presented, the nMOS transistor is created in the p-type substrate, and the pMOS transistor is created in the n-well, which is built-in into the p-type substrate. In the twin-tub CMOS technology, additional tubs of the same type as the substrate can also be created for device optimization. The simplified process sequence for the fabrication of CMOS integrated circuits on a p- type silicon substrate is shown in Fig. 2.1. 1/23/2016BVM ET5
6. Introduction Figure-2.1: Simplified process sequence for fabrication of the n-well CMOS integrated circuit with a single polysilicon layer, showing only major fabrication steps. 1/23/2016BVM ET6
7. Introduction The process starts with the creation of the n-well regions for pMOS transistors, by impurity implantation into the substrate. Then, a thick oxide is grown in the regions surrounding the nMOS and pMOS active regions. The thin gate oxide is subsequently grown on the surface through thermal oxidation. These steps are followed by the creation of n+ and p+ regions (source, drain and channel-stop implants) and by final metallization (creation of metal interconnects). 1/23/2016BVM ET7
8. Introduction The process flow sequence pictured in Fig. 2.1 may at first seem to be too abstract, since detailed fabrication steps are not shown. To obtain a better understanding of the issues involved in the semiconductor fabrication process, we first have to consider some of the basic steps in more detail. 1/23/2016BVM ET8
9. Fabrication Process flow: Basic steps Note that each processing step requires that certain areas are defined on chip by appropriate masks. Consequently, the integrated circuit may be viewed as a set of patterned layers of doped silicon, polysilicon, metal and insulating silicon dioxide. In general, a layer must be patterned before the next layer of material is applied on chip. The process used to transfer a pattern to a layer on the chip is called lithography. Since each layer has its own distinct patterning requirements, the lithographic sequence must be repeated for every layer, using a different mask. 1/23/2016BVM ET9
10. Fabrication Process flow: Basic steps To illustrate the fabrication steps involved in patterning silicon dioxide through optical lithography, let us first examine the process flow shown in Fig. 2.2. The sequence starts with the thermal oxidation of the silicon surface, by which an oxide layer of about 1 micrometer thickness, for example, is created on the substrate (Fig. 2.2(b)). The entire oxide surface is then covered with a layer of photoresist, which is essentially a light- sensitive, acid-resistant organic polymer, initially insoluble in the developing solution (Fig. 2.2(c)). 1/23/2016BVM ET10
11. Fabrication Process flow: Basic steps Figure-2.2: Process steps required for patterning of silicon dioxide. 1/23/2016BVM ET11
12. Fabrication Process flow: Basic steps If the photoresist material is exposed to ultraviolet (UV) light, the exposed areas become soluble so that the they are no longer resistant to etching solvents. To selectively expose the photoresist, we have to cover some of the areas on the surface with a mask during exposure. Thus, when the structure with the mask on top is exposed to UV light, areas which are covered by the opaque features on the mask are shielded. In the areas where the UV light can pass through, on the other hand, the photoresist is exposed and becomes soluble (Fig. 2.2(d)). 1/23/2016BVM ET12
13. Fabrication Process flow: Basic steps The type of photoresist which is initially insoluble and becomes soluble after exposure to UV light is called positive photoresist. The process sequence shown in Fig. 2.2 uses positive photoresist. There is another type of photoresist which is initially soluble and becomes insoluble (hardened) after exposure to UV light, called negative photoresist. If negative photoresist is used in the photolithography process, the areas which are not shielded from the UV light by the opaque mask features become insoluble, whereas the shielded areas can subsequently be etched away1/23/2016BVM ET13
14. Fabrication Process flow: Basic steps Negative photoresists are more sensitive to light, but their photolithographic resolution is not as high as that of the positive photoresists. Therefore, negative photoresists are used less commonly in the manufacturing of high-density integrated circuits. Following the UV exposure step, the unexposed portions of the photoresist can be removed by a solvent. Now, the silicon dioxide regions which are not covered by hardened photoresist can be etched away either by using a chemical solvent (HF acid) or by using a dry etch (plasma etch) process (Fig. 2.2(e)). 1/23/2016BVM ET14
15. Fabrication Process flow: Basic steps Figure-2.2: Process steps required for patterning of silicon dioxide. 1/23/2016BVM ET15
16. Fabrication Process flow: Basic steps Note that at the end of this step, we obtain an oxide window that reaches down to the silicon surface (Fig. 2.2(f)). The remaining photoresist can now be stripped from the silicon dioxide surface by using another solvent, leaving the patterned silicon dioxide feature on the surface as shown in Fig. 2.2(g). The sequence of process steps illustrated in detail in Fig. 2.2 actually accomplishes a single pattern transfer onto the silicon dioxide surface, as shown in Fig. 2.3. The fabrication of semiconductor devices requires several such pattern transfers to be performed on silicon dioxide, polysilicon, and metal. The basic patterning process used in all fabrication steps, however, is quite similar to the one shown in Fig. 2.2. 1/23/2016BVM ET16
17. Fabrication Process flow: Basic steps Also note that for accurate generation of high- density patterns required in sub-micron devices, electron beam (E-beam) lithography is used instead of optical lithography. In the following, the main processing steps involved in the fabrication of an n-channel MOS transistor on p-type silicon substrate will be examined. 1/23/2016BVM ET17
18. Fabrication Process flow: Basic steps Figure-2.3: The result of a single lithographic patterning sequence on silicon dioxide, without showing the intermediate steps. Compare the unpatterned structure (top) and the patterned structure (bottom) with Fig. 2.2(b) and Fig. 2.2(g), respectively. 1/23/2016BVM ET18
19. Fabrication Process flow: Basic steps 1/23/2016BVM ET19 The process starts with the oxidation of the silicon substrate (Fig. 2.4(a)),
20. Fabrication Process flow: Basic steps 1/23/2016BVM ET20 In which a relatively thick silicon dioxide layer, also called field oxide, is created on the surface (Fig. 2.4(b)).
21. Fabrication Process flow: Basic steps 1/23/2016BVM ET21 Then, the field oxide is selectively etched to expose the silicon surface on which the MOS transistor will be created (Fig. 2.4(c)).
22. Fabrication Process flow: Basic steps 1/23/2016BVM ET22 Following this step, the surface is covered with a thin, high-quality oxide layer, which will eventually form the gate oxide of the MOS transistor (Fig. 2.4(d)).
23. Fabrication Process flow: Basic steps 1/23/2016BVM ET23 On top of the thin oxide, a layer of polysilicon (polycrystalline silicon) is deposited (Fig. 2.4(e)).
24. Fabrication Process flow: Basic steps 1/23/2016BVM ET24 Polysilicon is used both as gate electrode material for MOS transistors and also as an interconnect medium in silicon integrated circuits. Undoped polysilicon has relatively high resistivity. The resistivity of polysilicon can be reduced, however, by doping it wi